A R C H I V E S O F M E T A L L U R G Y A N D M A T E R I A L S
Volume 58 2013 Issue 2
A. KIEBUS, M. STOPYRA, R. JAROSZ
INFLUENCE OF SAND-CASTING PARAMETERS ON MICROSTRUCTURE AND PROPERTIES OF MAGNESIUM ALLOYS
WPYW PARAMETRW ODLEWANIA GRAWITACYJNEGO NA MIKROSTRUKTUR I WACIWOCI STOPW MAGNEZU
The paper present the influence of modifying process on chemical composition, microstructure, and selected properties ofMg alloys. Two sand-casting creep-resistant alloys, Elektron 21 and WE43, were analyzed in various forms: without modifiers,with the amount of modifier suggested by the producer, and with this amount increased by 50% and 100%. The volumefraction of eutectic areas, tensile strength, and yield strength were measured and the fluidity and linear contraction wereanalyzed. The research shows that, in contrast to what is widely assumed to be a positive influence of rare-earth elementson Mg alloys properties, a large increase in the amount of modifiers does not always lead to an improvement in the alloyproperties. However, the results are tentative because they may have been influenced by the melting technology used, whichcan be improved. Rare-earth elements tend to react with fluxes, which could lead to a decrease in mechanical properties andfluidity. More research is planned wherein the alloys are melted under a protective atmosphere.
Keywords: Mg alloys, sand casting, modification, Elektron 21, WE43, properties, fluidity
W artykule zaprezentowano wpyw modyfikacji odlewniczych stopw magnezu na skad chemiczny, mikrostruktur iwybrane waciwoci. Badano 2 stopy odlewane do form piaskowych, przeznaczone do pracy w podwyszonej temperaturze:Elektron 21 i WE43 w czterech wariantach: bez modyfikacji, z iloci modyfikatorw dodan zgodnie z procedur zaleca-n przez producenta, powikszon o 50 i 100%. Wykonano ilociow analiz udziau objtociowego eutektyk, zmierzonowytrzymao na rozciganie, granic plastycznoci, wykonano prb lejnoci oraz skurczu liniowego. Wykazano, e mimopowszechnie uznanego za pozytywny wpywu metali ziem rzadkich na waciwoci stopw Mg dodawanie zwikszonych ilocimodyfikatorw w stosunku do zalece producentw nie zawsze ma dobry wpyw na wyniki. Prawdopodobnie duy wpywna wyniki bada miaa technologia odlewania, wymagajca poprawy zastosowane topniki mog reagowa z pierwiastkamistopowymi i powodowa obnienie waciwoci mechanicznych i lejnoci. W przyszoci planowane s podobne badania dlastopw topionych w atmosferze gazowej.
Magnesium is the lightest metal used for constructionalalloys. Magnesium alloys are characterized by low density andgood mechanical properties , which are the primary reasonsthat they find widespread use in the motor vehicle and aircraftindustries. The disadvantages of these alloys are their poorproperties at elevated temperature  and their high reactivity. A range of alloys are commercially available, from Mg-Alalloys to the highest strength, high-temperature Mg-Zr alloyswith the addition of yttrium. However, alloys that contain areexpensive due to difficulties in casting. Therefore, a need existsfor an alternative alloy with properties similar to Mg-Y alloys,but with foundry handling and associated costs similar to thatof non-yttrium-containing alloys .
The basic function of rare-earth (RE) chemical elementsis formation of reinforcing intermetallic phases that remainstable at elevated temperature . Simultaneously, they limitthe range of crystallization temperature, which in turn decreas-
es hot cracking susceptibility, improving its welding proper-ties . Alloys containing gadolinium are characterized bytheir substantial age-hardening properties. Neodymium cre-ates phases both within the solid-solution grains as well as atthe boundary of the solid solution of -Mg, influencing thereinforcing effect of age hardening by minimizing the rangeof solubility of gadolinium in an -Mg solid solution. Thisfacilitates the process of age hardening with a lower contentof gadolinium [6,7], which is expensive. However, gadoliniumtends to segregate (and this tendency increases with increasingcontent), which decreases the alloys ductility .
In sand-casting magnesium alloys, the one of the basicalloy additions is zirconium (it is absent only in Mg-Al alloys).Its basic task is to refine -Mg solid solution. This effect isattributed to the similar crystal lattices of Mg and Zr .Zinc is another element that is added to magnesium alloysto improve their mechanical properties during heat treatment.In addition, it increases the resistance to corrosion caused byimpurities such as Fe and Ni [4, 9]. In magnesium alloys
SILESIAN UNIVERSITY OF TECHNOLOGY, KATOWICE, POLAND ZM WSK RZESZW, POLAND
containing Nd and Gd, the addition of Zn inhibits the ageingeffect . The addition of yttrium increases creep resistance,thereby enabling age hardening, which stems from the factthat the Mg-Y intermetallic phases are characterized by a lowdiffusion rate and good coherence with the alloys matrix .
To obtain the appropriate chemical composition,fine-grained structure and good properties, a process of mod-ification is introduced. This paper presents the results of re-search into the amounts of casting modifiers that should beintroduced into the alloy and the influence of these modifierson the chemical composition, microstructure, and mechanicaland technological properties of WE43 and Elektron 21 alloys.
2. Research material
Two sand-casting magnesium alloys were investigated:WE43 and Elektron 21. The modifier used in this case goesunder the commercial name of Zirmax, with the addition of agadolinium and neodymium hardeners for Elektron 21 and aWE hardener for the WE43 alloy. The chemical compositionsof the alloys used are presented in Table 1, with a list ofmodifiers presented in Table 2.
3. Methodology of research
The alloys were melted in a gas furnace using a steel St3Smelting crucible with a capacity of 30 kg. The sequence oftesting stages was as follows:1. Load ingots into the crucible;2. Heat alloy to 740-780C until melting is complete;3. Remove oxides from the surface, add Zirmax modifier and
appropriate hardeners. The options or variations used inthe modification process are presented in Tables 3 and 4.
4. Heat alloy to 780 to 800C, mix, and cast into molds.
TABLE 1Chemical composition of WE43 and Elektron 21 alloys [wt%]
Nd Y Zr Zn Gd Mn Fe Ag Mg
WE43 - 1.12 2.3 4.1 0.49 0.01 - 0.01 0.001
The chemical composition was deduced from awavelength-dispersive analysis of the x-ray fluorescence spec-trum (WDXRF) using a Bruker S4 EXPLORER. Typicaletchants for Mg alloys were used. The microstructure of themagnesium alloys was observed with an OLYMPUS GX 71metallographic microscope and a HITACHI S-3400N scan-ning electron microscope equipped with the Thermo Noranenergy-dispersion spectrometer. Phase composition was ana-lyzed using JEOL JDX-7S diffractometer equipped with a cop-per anode (CuK = 1.5406 A
). Phases were indentyfied with
the help of pcpdfwin, version 2.1 (JCPDS-ICDD). Quantita-tive analysis of the microstructure was done with the Met-Iloprogram.
4. Results and discussion
4.1. Microstructure of WE43 and Elektron 21 in as-castcondition
WE43 alloyAfter sand casting, -Mg solid-solution matrix and eu-
tectic areas were observed in the structure of the WE43 al-loy (Fig. 4a). The intermetallic phase is isomorphic to theMg5Gd phase. In addition, precipitations containing yttrium(Fig. 4b) occur close to the eutectic areas-most probably Mg2Yor MgY phases.
Fig. 4. Microstructure of WE43 magnesium alloy in as-cast condition:(a) scanning electron microscope, (b) scanning transmission electronmicroscope
Elektron 21 alloyThe Elektron 21 alloy is characterized by an -Mg
solid-solution structure with eutectic areas at the grain bound-aries of the -Mg solid solution (Fig. 5a) and regularly shapedprecipitates of a phase containing gadolinium (Fig. 5b). Thephase that, together with the solid solution, forms the eutecticareas is the Mg3Gd phase, whereas the minor precipitates arethe MgGd3 phase.
Fig. 5. Microstructure of Elektron 21 alloy in as-cast condition: (a)scanning electron microscope, (b) transmission electron microscope
4.2. Microstructure of introduced modifiers andhardeners
The microstructure of hardeners consists of the -Mgsolid solution with one or more intermetallic phases. In theNd hardener (Fig. 6), the intermetallic phase precipitate atthe -Mg solid-solution grain boundary and within grains.It contains about 30% neodymium. The phase was identifiedas Mg12Nd. Moreover, singular precipitates containing 55%neodymium were also observed.
Fig. 6. Diversified morphology of Mg12Nd phase precipitates withinmicrostructure of Nd hardener: (a) Light microscope, (b) ScanningElectron Microscope, back-scattered electron image
The gadolinium hardener includes phase precipitates con-taining approximately 50% Gd, which forms the eutectic withthe -Mg solid solution. This is a type of Mg5Gd phase. More-over, small amounts of phase precipitates containing approxi-mately 65% Gd were present (Fig. 7).
Fig. 7. Mg5Gd phase precipitates in microstructure of Gd hardener:(a) LM, (b) SEM BSE image
Phase precipitates containing approximately 30% Y and10% REs were observed in the -Mg solid-solution matrix ofthe WE hardener. Further small precipitates containing almostpure yttrium were also observed (Fig. 8). The phase containingY and REs was identified as Mg24Y5 phase, and the precipi-tates containing almost pure yttrium was identified as the -Ysolid solution.
The Zirmax modifier is characterized by a dual-phase mi-crostructure composed of -Mg solid solution a